1 Wang et al. Nanoscale Research Letters (2015) 10:280 DOI /s NANO EXPRESS Facile Synthesis of Mn-Doped ZnO Porous Nanosheets as Anode Materials for Lithium Ion Batteries with a Better Cycle Durability Linlin Wang 1,2, Kaibin Tang 2*, Min Zhang 1 and Jingli Xu 1* Open Access Abstract Porous Zn 1 x Mn x O(x = 0.1, 0.2, 0.44) nanosheets were prepared by a low-cost, large-scale production and simple approach, and the applications of these nanosheets as an anode material for Li-ion batteries (LIBs) were explored. Electrochemical measurements showed that the porous Zn 0.8 Mn 0.2 O nanosheets still delivered a stable reversible capacity of 210 ma h g 1 at a current rate of 120 ma g 1 up to 300 cycles. These results suggest that the facile synthetic method of producing porous Zn 0.8 Mn 0.2 O nanostructure can realize a better cycle durability with stable reversible capacity. Keywords: Mn-doped ZnO; Porous nanosheets; Li-ion batteries Background ZnO, as 3d a transition-metal oxide, has been considered as an anode material for Li-ion batteries (LIBs) due to the following characteristics: high specific capacity (978 ma h g 1 ), abundance, low cost, non-toxic, easily produced, and chemically stable [1 5]. However, it often suffers the loss of capacity upon the cycling due to drastic volume changes during the formation of lithium zinc alloys [6 8]. Therefore, a lot of effort has been devoted to overcome these problems; correspondingly, many methods have been developed, such as (i) preparing ordered nanostructured materials [2, 9]; (ii) incorporating with Ni 3 ZnC 0.7 ; (iii) coating with Ni, C, and CoO-C layers [6, 11, 12]; and (iv) doping with Mg . These techniques enhance the conductivity, facilitate the lithiation/delithiation process, or buffer the volume changes. For example, Ping et al. reported Zn 1 x Mg x O (x = 0, 0.18) thin films showed an improved cycling stability compared to that of ZnO thin films. The doped Mg ions may only act as a buffer in a form of MgO to alleviate the stress caused by the volume changes during the formation of lithium zinc alloys . * Correspondence: 2 Department of Chemistry, University of Science and Technology of China, Hefei , P.R. China 1 School College of Chemistry and Chemical Engineering, Shanghai University of Engineering Science, 333 Longteng Road, Shanghai , P.R. China Mn-doped ZnO has been widely investigated for their optical properties, magnetic properties, and sensing properties [14 18]. However, it has rarely been used as anode materials in LIBs. In this work, we successfully synthesized porous Zn 1 x Mn x O (x = 0.1, 0.2, 0.44) nanosheets in high yield using a facile method. The electrode performance of the samples was electrochemically investigated, and the representative as-synthesized Zn 1 x Mn x O(x = 0.2) exhibited a better cycle durability with stable reversible capacity of 210 ma h g 1 for up to 300 cycles at 120 ma g 1. Methods 1. ZnO precursor synthesis The ZnO precursor was prepared by our previous reported method . The ZnCl 2 5H 2 O (10.0 mmol) and C 6 H 8 O 7 H 2 O (6.7 mmol) were dissolved in 10-mL water, then solid NaOH (50.0 mmol) was directly added into the mixture solution. Subsequently, 40 ml of distilled water was added and a precursor solution was obtained after 10 min. The white precipitate (flower-like ZnO) was obtained. 2. Synthesis of Zn 1 x Mn x O 2015 Wang et al. This is an Open Access article distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/4.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly credited.
2 Wang et al. Nanoscale Research Letters (2015) 10:280 Page 2 of 5 In a typical process, the obtained ZnO (2.0 mmol) was immersed into Mn(Ac) 2 4H 2 O (0.2 M, 20 ml) aqueous solution and 40 ml of water was added, stirring for 4 days at room temperature. Then, the resulting powders were obtained and washed with distilled water and ethanol several times, dried at 60 C. Following, the resulting powders were kept at 350 C for 3 h under argon atmosphere and the target product Zn 1 x Mn x O (x = 0.2) was obtained (denoted as sample A). In addition, Zn 1 x Mn x O(x =0.1, 0.44) was also obtained with Mn(Ac) 2 4H 2 O with the amount 8 and 30 ml, respectively (denoted as sample B and sample C). 3. Characterization The as-prepared particles were characterized by powder X-ray diffraction (XRD) on a Philips X pert X-ray diffractometer equipped with Cu Kα radiation (λ = Å). The morphologies of the samples were examined on a field-emission scanning electron microscopy (FESEM; JEOL JSM-6700 F) and a transmission electron microscopy (TEM; JEOL-2010). The HRTEM images were taken on an aberration-corrected analytical transmission electron microscopy (ARM200F). N 2 adsorption desorption isotherms were measured on a Micromeritics ASAP-2000 nitrogen adsorption apparatus at 150 K. The electrodes for electrochemical testing consisted of 70 wt% active materials, 15 wt% conductive material (acetylene black), and 15 wt% binder (polyvinylidene fluoride (PVDF)). Test cells (2016) were assembled in glove box using lithium metal as the anode, Celgard 2600 as the separator, and 1 M LiPF 6 in ethylene carbonate and dimethyl carbonate solution (v/v, 1:1). The galvanostatical charge/discharge measurement was carried out by a LAND-CT2001 battery cycler (Wuhan, China) testing system in the voltage range of V (vs. Li/Li + ). Results and Discussion The XRD pattern of the precursor is shown in Fig. 1a. All of the peaks can be assigned to hexagonal ZnO (JCPDS file No ). The chemical composition of the sample A was determined by XRD and XPS. The crystallinity and crystal phase of the sample A were demonstrated by the XRD shown in Fig. 1b. The peaks in the diffraction pattern of Zn 1 x Mn x O at 31.81, 34.43, and can be indexed to a hexagonal wurtzite structure, which consists of three prominent peaks corresponding to (100), (002), and (101) planes, respectively. Compared with the peak position of ZnO (inset), that of Zn 1 x Mn x O was found to shift towards lower angles with Mn incorporation, probably due to the larger ionic radius of Mn 2+ (0.066 nm) relative to that of Zn 2+ (0.060 nm) [20, 21]. The XPS survey spectrum confirms that the sample mainly contains Zn, Mn, and O (Fig. 2). Fig. 1 a The XRD pattern of the ZnO; b the XRD pattern of the sample Aandinset is an enlarged picture of XRD peaks appearing at ~30 40 The strong peaks at around ev (Fig. 2a) are assigned to Mn2p3/2. The values correspond to a binding energy of Mn 2+ ion . The peak at ev (Fig. 2c) is assigned to Zn2p3/2 for the Zn 2+ state (Fig. 2b) and the peak at ev (Fig. 2c) corresponds to the binding energy of O1s. In addition, the ratio of Mn to Zn of 6.38:25.05 is given by the quantification of peaks, indicating that the molar ratio of Mn to Zn is near 1:4. The above results indicate that the prepared sample A is single phase Zn 0.8 Mn 0.2 O. The SEM images (Fig. 3a, b) show that the Zn 0.8 Mn 0.2 O samples are sheet-like morphology with many holes in the nanosheets. From the TEM images (Fig. 3c e), the porous nanosheets were clearly observed, which further confirms the formation of Zn 0.8 Mn 0.2 O porous nanostructures. We also examined the phase purity of the resulting powder that has not been calcined by the XRD. From the XRD Fig. 2 XPS spectra of the sample A: a Mn2p3/2, b Zn2p3/2, and c O1s
3 Wang et al. Nanoscale Research Letters (2015) 10:280 Page 3 of 5 Fig. 3 SEM images of the sample A: a low magnification, b high magnification; TEM images: c low magnification and d, e high magnification; (f) a HRTEM image pattern (Additional file 1: Figure S1 in supporting information), it is clearly seen that the diffraction pattern of the resulting powder are different from the precursor ZnO and Zn 1 x Mn x O. This result suggests that the chemical reaction process (Mn-doped ZnO) is not simple zinc substituted by manganese but involves a complex reaction which led to its structure and composition being changed. The structure and composition of the resulting powder is complex and difficult to identify. However, due to the similar XRD pattern of Zn(OH) 2 and ZnO, it is reasonable that hydroxide ions might be introduced into the resulting powder during the reaction process, in addition to the possible organic molecules. The morphology of resulting powder (Additional file 1: Figure S2) is nanosheets.
4 Wang et al. Nanoscale Research Letters (2015) 10:280 Page 4 of 5 Fig. 4 Schematic illustration of the synthesis process of the Zn 1 x Mn x O nanosheets Interestingly, after calcination, a number of pores appear on the nanosheets, possibly due to decomposition of the organic molecules and hydroxyl group in the calcination process. The pore size distribution curves have been investigated by using Barrett Joyner Halenda (BJH) method. Basing on the report of nitrogen adsorption desorption shown in Additional file 1: Figure S3, the Zn 0.8 Mn 0.2 O exhibited a BET surface area of m 2 g 1 and adsorption average pore diameter of 8.5 nm. For the Zn 0.8 Mn 0.2 O nanosheets, lattice images showed fringes with a spacing of ca nm and ca nm, corresponding to the (110) and (002) planes of ZnO (Fig. 3f). An overall schematic model of the synthesis procedure is shown in Fig. 4. The energy dispersion X-ray spectrum (EDS) of the as-prepared sample B and C (Additional file 1: Figure S4) shows that the molar ratio of Mn to Zn of 7.99:66.12 and 16.66:20.96 is near 1:8 (Zn 0.9 Mn 0.1 O) and 1:1.25 (Zn 0.56 Mn 0.44 O), respectively. The electrochemical properties of the porous Zn 0.8 Mn 0.2 O nanosheets (sample A) were characterized by a galvanostatic method. Figure 5a, b shows first charge/discharge profiles and cycling performance of the Zn 0.8 Mn 0.2 O electrode tested in the potential range of 0.01 to 3.0 V and at a current density of 120 ma h g 1. The Zn 0.8 Mn 0.2 O nanosheets exhibit the initial discharge and charge capacities of 1198 and 763 ma h g 1, with an initial coulombic efficiency of 64 %. After 50 cycles, this Zn 0.8 Mn 0.2 Oelectrode delivers a reversible capacity of 340 ma h g 1. Even at 300 cycles, this Zn 0.8 Mn 0.2 O material still retains a stable capacity of 210 ma h g 1, thus exhibiting an excellent cycle durability. For comparison purposes, we also investigate the electrochemical properties of sample B, sample C, and the ZnO precursor (Fig. 5b). Sample B retains a reversible capacity of ~220 ma h g 1 up to 50 cycle, and the sample delivers a lower capacity of ~90 ma h g 1, while the capacity of the ZnO deteriorates severely and ZnO delivers a much lower capacity of 64 ma h g 1 up to 50 cycles. Apparently, the reversible capacity of the Zn 0.8 Mn 0.2 O porous nanosheets is enhanced than that of sample B, sample C, and the precursor ZnO. The good cycle durability of the Zn 0.8 Mn 0.2 Omaterial might be reasonable to be attributed to the fact that a great number of the cavities among nanosheets are all Fig. 5 a Initial discharge/charge profile for the Zn 0.8 Mn 0.2 O; b cycling performances and Coulombic efficiencies of the Zn 1 x Mn x O and ZnO electrodes
5 Wang et al. Nanoscale Research Letters (2015) 10:280 Page 5 of 5 beneficial to relieve the strain induced by the severe volume variations of Zn 0.8 Mn 0.2 OduringLi + uptake release, which might improve better rate capacity and the cycling performance. Conclusions In conclusion, the Mn-doped ZnO porous nanosheets were successfully synthesized by a simple approach and their electrochemical performance were evaluated. The obtained Zn 0.8 Mn 0.2 O porous nanosheets exhibit better cycle durability with good reversible capacity. The cavities among nanosheets maybe could effectively suppress the volume expansion during cycling and enhances the electric conductivity of electrodes, etc., giving rise to better electrochemical performance and cycling stability. In addition, our results provide a simple, effective strategy to fabricate the Zn 0.8 Mn 0.2 O nanostructure. Additional File Additional file 1: The XRD pattern of three samples, SEM image of the resulting power, Nitrogen adsorption/desorption isotherms and pore size distribution of Zn 0.8 Mn 0.2 O and EDS spectrum of the products. Figure S1. XRD pattern of three samples, Figure S2. SEM image of the resulting power, Figure S3. Nitrogen adsorption/desorption isotherms and pore size distribution (inset) of Zn 0.8 Mn 0.2 O (sample A). Figure S4. EDS spectrum of the products (a) sample B; (b) sample C. Competing Interests The authors declare that they have no competing interests. Authors Contributions LLW prepared the manuscript and carried out the experiment. KBT helped in the technical support for the characterizations and design of the experiment. MZ and JLX participated in the experiment. All the authors discussed the results and approved the final manuscript. Acknowledgements This work was supported by the Yang Fan project of Science and Technology Commission of Shanghai Municipality (No.14YF ) and the Young Teacher Training Scheme of Shanghai (No. ZZgcd14008) and the National Natural Science Foundation of China (No , No , No ). 6. Zhang CQ, Tu JP, Yuan YF, Huang XH, Chen XT, Mao F. Electrochemical performances of Ni-coated ZnO as an anode material for lithium-ion batteries. J Electrochem Soc. 2007;154:A Belliard F, Irvine JTS. Electrochemical performance of ball-milled ZnO-SnO 2 systems as anodes in lithium-ion battery. J Power Sources. 2001;97 98: Zheng F, Feng H, Ye Z, Yue C, Zong QQ. The electrochemical reaction of zinc oxide thin films with lithium. J Electrochem Soc. 2003;150:A Liu J, Li Y, Huang X, Li G, Li Z. Layered double hydroxide nano- and microstructures grown directly on metal substrates and their calcined products for application as Li-ion battery electrodes. Adv Funct Mater. 2008;18: Tang XD, Pan QM, Liu J. Enhancing lithium storage capacity of ZnO anodes through Ni 3 ZnC 0.7 incorporation. J Electrochem Soc. 2010;157:A Liu J, Li Y, Ding R, Jiang J, Hu Y, Ji X, et al. Carbon/ZnO nanorod array electrode with significantly improved lithium storage capability. J Phys Chem C. 2009;113: Zhao W, Li QM, Qin PM. Fabrication and electrochemical behavior of flower-like ZnO-CoO-C nanowall arrays as anodes for lithium-ion batteries. J Alloys Compd. 2011;509: Yan GF, Fang HS, Li GS, Li LP, Zhao HJ, Yang Y. Improved electrochemical performance of Mg-doped ZnO thin film as anode material for lithium ion batteries. Chin J Struct Chem. 2009;28: Ruan HB, Fang L, Li DC, Saleem M, Qin GP, Kong CY. Effect of dopant concentration on the structural, electrical and optical properties of Mn-doped ZnO films. Thin Solid Films. 2011;519: Xin M, Hu LZ, Liu DP, Yu NS. Effect of Mn doping on the optical, structural and photoluminescence properties of nanostructured ZnO thin film synthesized by sol-gel technique. Superlattice Microst. 2014;74: Du SP, Zhao CW, Luo BC, Xing H, Jin KX, Chen CL. Effect of Li-doping on the structure and electrical and magnetic properties of Mn-ZnO film. Rare Metal Mat Eng. 2013;42: Kim JH, Lee JB, Kim H, Choo WK, Ihm Y, Kim D. Electrical and magnetic properties of Mn-doped ZnO. Ferroelectrics. 2002;273: Mao Y, Ma S, Li X, Wang C, Li F, Yang X, et al. Effect of Mn doping on the microstructures and sensing properties of ZnO nanofibers. Appl Sur Sci. 2014;298: Wang LL, Zhao DL, Zhang M, Wang CH, Tang KB, Zhang XZ, et al. Zn 0.5 Co 0.5 O solid solution nanoparticles with durable life for rechargeable lithium-ion batteries. Nano LIFE. 2014;4: (7 pages). 20. Milenova K, Avramova I, Eliyas A, Blaskov V, Stambolova I, Kassabova N. Application of activated M/ZnO (M = Mn, Co, Ni, Cu, Ag) in photocatalytic degradation of diazo textile coloring dye. Environ Sci Pollut R. 2014;21: Ahmad M, Ahmed E, Ahmed W, Elhissi A, Hong ZL, Khalid NR. Enhancing visible light responsive photocatalytic activity by decorating Mn-doped ZnO nanoparticles on grapheme. Ceram Int. 2014;40: Received: 26 April 2015 Accepted: 16 June 2015 References 1. Xie Q, Ma Y, Zhang X, Wang L, Yue G, Peng DL. ZnO/Ni/C composite hollow microspheres as anode materials for lithium ion batteries. J Alloys Compd. 2015;619: Xiao L, Mei D, Cao M, Qu D, Deng B. Effects of structural patterns and degree of crystallinity on the performance of nanostructured ZnO as anode material for lithium-ion batteries. J Alloys Compd. 2015;627: Zhu J, Zhang G, Gu S, Lu B. SnO 2 nanorods on ZnO nanofibers: a new class of hierarchical nanostructures enabled by electrospinning as anode material for high-performance lithium-ion batteries. Electrochim Acta. 2014;150: Yue HY, Shi ZP, Wang QX, Cao ZX, Dong HY, Qiao Y, et al. MOF-derived cobalt-doped composites as a high-performance anode material for lithium-ion batteries. Acs Appl Mater Inter. 2014;6: Wu MS, Chang HW. Self-assembly of NiO-coated ZnO nanorod electrodes with core shell nanostructures as anode materials for rechargeable lithium-ion batteries. J Phys Chem C. 2013;117: Submit your manuscript to a journal and benefit from: 7 Convenient online submission 7 Rigorous peer review 7 Immediate publication on acceptance 7 Open access: articles freely available online 7 High visibility within the field 7 Retaining the copyright to your article Submit your next manuscript at 7 springeropen.com
Man et al. Nanoscale Research Letters (2015) 10:279 DOI 10.1186/s11671-015-0974-4 NANO EXPRESS Graphene-Based Flexible and Transparent Tunable Capacitors Open Access Baoyuan Man 1*,ShicaiXu 1,2, Shouzheng
Crystalline Silver Nanowires by Soft Solution Processing NANO LETTERS 2002 Vol. 2, No. 2 165-168 Yugang Sun, Byron Gates, Brian Mayers, and Younan Xia* Department of Chemistry, UniVersity of Washington,
One-Dimensional Nanostructures: Synthesis, Characterization, and Applications** By Younan Xia,* Peidong Yang,* Yugang Sun, Yiying Wu, Brian Mayers, Byron Gates, Yadong Yin, Franklin Kim, and Haoquan Yan
Chem. Rev. 2005, 105, 1103 1169 1103 Self-Assembled Monolayers of Thiolates on Metals as a Form of Nanotechnology J. Christopher Love, Lara A. Estroff, Jennah K. Kriebel, Ralph G. Nuzzo,*, and George M.
Patterning: Principles and Some New Developments** By Matthias Geissler and Younan Xia* This article provides an overview of various patterning methodologies, and it is organized into three major sections:
Reaction of Aluminum with Water to Produce Hydrogen A Study of Issues Related to the Use of Aluminum for On-Board Vehicular Hydrogen Storage U.S. Department of Energy Page 1 of 26 CONTENTS EXECUTIVE SUMMARY..
Chin.J.Geochem.(2014)33:024 044 DOI: 10.1007/s11631-014-0657-3 Scientific data and their release of Chang E-1 and Chang E-2 ZUO Wei, LI Chunlai *, and ZHANG Zhoubin The Science and Application Center for
Properties of Electrons, their Interactions with Matter and Applications in Electron Microscopy By Frank Krumeich Laboratory of Inorganic Chemistry, ETH Zurich, Vladimir-Prelog-Weg 1, 8093 Zurich, Switzerland
Chem. Rev. 1990, 90. 33-72 93 The Sol-Gel Process LARRY L. HENCH' and JON K. WEST Dq"nt of Materials Sc*mce and Enghwrhg, Advanced Materials Research Center, UnimrMy of Floryle. oakresville. Fknm 326 11
Single-Electron Devices and Their Applications KONSTANTIN K. LIKHAREV, MEMBER, IEEE Invited Paper The goal of this paper is to review in brief the basic physics of single-electron devices, as well as their
T H I R D E D I T I O N Investigating Matter Through Inquiry A project of the American Chemical Society Education Division Office of K 8 Science American Chemical Society American Chemical Society Inquiry
About the Department of Energy s Basic Energy Sciences Program Basic Energy Sciences (BES) supports fundamental research to understand, predict, and ultimately control matter and energy at the electronic,
Journal of Experimental Nanoscience, Vol. 2, Nos. 1 2, March June 2007, 3 11 Arrays of Cu 21 -complexed organic clusters grown on gold nano dots A. HATZOR-DE PICCIOTTO*yz, A. D. WISSNER-GROSSz, G. LAVALLEEz
i Acid-base Chemistry of Aquatic Systems An introduction to the chemistry of acid-base equilibria with emphasis on the carbon dioxide system in natural waters eith A. Hunter Professor in Chemistry Department
DRINKING WATER THROUGH RECYCLING The benefits and costs of SUPPLying direct to the distribution system A REPORT OF A STUdy BY THE AUSTRALIAN ACADEMY OF TEChnOLOGICAL SCIENCES And ENGINEERING (ATSE) DRINKING
Process monitoring in biogas plants Bernhard Drosg Technical Brochure written by: Bernhard Drosg Copyright 2013 IEA Bioenergy. All rights reserved. First electronic edition produced in 2013 A catalogue
LHC Project Note 78 / 97 January 18, 1997 firstname.lastname@example.org On Graphite Transformations at High Temperature and Pressure Induced by Absorption of the LHC Beam Jan M. Zazula CERN-SL/BT(TA) Keywords: Summary
JOURNAL OF MASS SPECTROMETRY J. Mass Spectrom. 21; 36: 849 865 SPECIAL FEATURE: TUTORIAL An introduction to quadrupole time-of-flight mass spectrometry Igor V. Chernushevich, Alexander V. Loboda and Bruce
Acid-base Equilibria and Calculations A Chem1 Reference Text Stephen K. Lower Simon Fraser University Contents 1 Proton donor-acceptor equilibria 4 1.1 The ion product of water... 4 1.2 Acid and base strengths...
Mattaini et al. Cancer & Metabolism (2015) 3:5 DOI 10.1186/s40170-015-0131-7 Cancer & Metabolism RESEARCH An epitope tag alters phosphoglycerate dehydrogenase structure and impairs ability to support cell
When Poor Solubility Becomes an Issue: From Early Stage to Proof of Concept S. Stegemann a, F. Leveiller b, D. Franchi c, H. de Jong d, H. Lindén e,* a Capsugel, Rijksweg 11, 2880 Bornem, Belgium b AstraZeneca,
Author Guidelines What to send and when At Submission Please consult individual journal guidelines for details of any additional required files. In general, initial manuscript submissions to Royal Society
INTERNATIONAL CONFERENCE ON HARMONISATION OF TECHNICAL REQUIREMENTS FOR REGISTRATION OF PHARMACEUTICALS FOR HUMAN USE ICH HARMONISED GUIDELINE GUIDELINE FOR ELEMENTAL IMPURITIES Q3D Current Step 4 version
Unit 8 Chemical Equilibrium Focusing on Acid-Base Systems unit 8Chemical Equilibrium Chemical Equilibrium Focusing on Acid Base Systems Equilibrium describes any condition or situation of balance. We recognize
All Biochars are Not Created Equal, and How to Tell Them Apart Version 2 (October 2009), which supercedes the digital reprint issued at the North American Biochar Conference, Boulder, CO August 2009 Hugh
AS/A Level GCE GCE Chemistry A OCR Advanced Subsidiary GCE in Chemistry A H034 OCR Advanced GCE in Chemistry A H434 version 4 September 2013 QAN 500/2425/5 QAN 500/2347/0 Contents 1 About these Qualifications
JOURNAL OF MASS SPECTROMETRY, VOL. 3, 1519È1532 (1995) SPECIAL FEATURE: TUTORIAL Principles and Instrumentation in Time-of-ýight Mass Spectrometry Physical and Instrumental Concepts Michael Guilhaus School
Two-Photon Absorption in ear-ir Conjugated Molecules: Design Strategy and Structure Property Relations lga V. Przhonska, Scott Webster, Lazaro A. Padilha, Honghua Hu, Alexey D. Kachkovski, David J. Hagan,
600 IEEE TRANSACTIONS ON SIGNAL PROCESSING, VOL. 45, NO. 3, MARCH 1997 Sparse Signal Reconstruction from Limited Data Using FOCUSS: A Re-weighted Minimum Norm Algorithm Irina F. Gorodnitsky, Member, IEEE,